In this work a novel antibacterial surface composed of an organic-inorganic hybrid matrix of tetraorthosilicate and a polyelectrolyte is presented. A precursor solution of tetraethoxysilane (TEOS) and poly(acrylic acid sodium salt) (PAA) was prepared and subsequently thin films were fabricated by the dip-coating technique using glass slides as substrates. This hybrid matrix coating is further loaded with silver nanoparticles using an in situ synthesis route. The morphology and composition of the coatings have been studied using UV-VIS spectroscopy and atomic force microscopy (AFM). Energy dispersive X-ray (EDX) was also used to confirm the presence of the resulting silver nanoparticles within the thin films. Finally the coatings have been tested in bacterial cultures of genus Lactobacillus plantarum to observe their antibacterial properties. It has been experimentally demonstrated that these silver loaded organic-inorganic hybrid films have a very good antimicrobial behavior against this type of bacteria.
Microbes and bacteria are the most abundant of all living organisms in our planet and a large of them are pathogens. Because of that, there is an enormous interest in the research of highly efficient and low cost antibacterial surface treatments and coatings to avoid the apparition of these microorganisms in instrumentals, devices, laboratories, operating rooms, etc. [1, 2].
Silver ions show a notorious broad spectrum biocide effect. There are several known mechanisms where the utilization of silver has led to an extraordinary toxicity for bacteria [3–6]. Moreover, silver is particularly attractive because it combines the high toxicity for bacteria with a low toxicity for humans [7–9]. Its disinfectant properties for hygienic and medicinal purposes are known since ancient times, and for example it has been extensively used to prevent wound infection since World War I .
Most of the approaches for achieving antibacterial surfaces are based on doping some elements with silver particles which act as silver ion source, for example, in textiles [11, 12], surgical instruments , and other surfaces . Some authors have reported how silver nanoparticles , nanorods , or nanotubes  are especially efficient antibacterial agents because of their large surface to volume ratio. Up to now such silver nanoparticles have been immobilized on inorganic porous hosts such as zeolites, calcium phosphate, and carbon fiber [18–20]. Moreover, silver-supported silica materials, such as silica glass , silica thin films , and silica nanoparticles , are also good candidates for antibacterial materials due to their fine chemical durability and high antibacterial activity. Moreover, a surface can obtain contact bacteria-killing capacity through chemical modification with tethered bactericidal functionalities such as quaternary amine compounds [24, 25], phosphonium salts , and titanium oxide particles , which are able to kill bacteria upon contact.
However, the biocide efficiency of such coatings depends on the ability of the trapped silver to release ions. Consequently, silver particles with a high specific area show more efficient ion release mechanisms and therefore the antibacterial effect is enhanced. There is a wide variety of coating techniques that have been used for fabricating antibacterial coatings, such as PVD , spin-coating , or electrospinning [30, 31]. In this work, we have developed a facile method to produce an organic-inorganic hybrid matrix by the sol-gel process using the dip-coating technique onto glass substrates. This approach allows to fabricate biocide films in a fast and simple way compared to other fabrication techniques .
Polymer-silica hybrid materials have drawn the attention of many researchers recently because of their compatibility with living matter and their promising applications in the medical field [33, 34]. Organic polymers in general enjoy a high flexibility, low density, toughness, and easy formability whereas ceramic materials possess other excellent mechanical properties such as a high hardness, combined with a good resistance to high temperature or strong solvents. In this work, these new class of materials are employed to obtain a porous silica surface containing uniformly distributed silver nanoparticles inside the coating. To our knowledge, this is the first time that TEOS/PAA hybrid matrices loaded with silver nanoparticles are fabricated. In addition, their possible antibacterial behavior is also studied.
In this work, the hybrid (organic/inorganic) precursor solution was prepared mixing a water-based solution of poly(acrylic acid sodium salt) (PAA), tetraethoxysilane (TEOS), and ethanol (EtOH). The PAA solution was prepared using ultrapure water (18.2 MΩcm) and its concentration was varied throughout the experiment, from 10-3 to 20·10-3 M respect to the repetitive unit. Silver nanoparticles were further in situ synthesized from silver nitrate and borane dimethylamine complex (DMAB). All chemicals were purchased from Sigma-Aldrich and used without any further purification.
For the bacterial cultures, MRS broth and MRS agar were provided from Fluka. Lactobacillus plantarum were obtained from CECT (The Spanish Type Culture Collection University of Valencia). These bacteria are gram-positive, rod, aerotolerant and belong to risk group I.
Fabrication of the thin films
A starting solution was prepared by mixing together TEOS, EtOH, and the water-based solution of PAA in the following weigh ratio (0.11:0.77:0.12). The pH of the solution was adjusted to 8 by adding NaOH dropwise. The chemicals were mixed under vigorous stirring and the final solution was aged for 30 min. Then the coatings were created by dip-coating. Glass slide substrates were immersed into the starting solution for 15 s and then the substrates were lifted from the solution at a speed of 0.4 mm/s. In order to evaporate very gently the remaining solvents and to allow the consolidation of the coating, samples were stored at room conditions for 3 h. Using this method, high quality transparent coatings were obtained.
Then, the hybrid coating was used as host for in situ silver nanoparticle synthesis. Silver ions were immobilized into the hybrid matrix by ion interchange by simply immersing the coated samples into a AgNO3 solution (10 × 10-3 M). During this loading immersion silver cations (Ag+) formed electrostatic pairs with some of the carboxylate groups from PAA. This loading step was carried out for 5 min. Afterwards the silver loaded into the coatings were reduced by immersing the samples into a 0.1 M dimethylamine borane (DMAB) solution which act as reducing agent. Therefore the carboxylate-bonded Ag+ ions were reduced to produce zero-valent silver (Ag0) particles. Between each loading and reduction step the samples were thoroughly rinsed in ultrapure water. This loading/reduction immersion cycle can be repeated as many times as desired to induce a growth of the silver nanoparticles .
Characterization of the coating film
Atomic force microscopy (AFM) was used to characterize the roughness and the surface morphology of the coating. The samples were scanned using a Veeco Innova AFM, in tapping mode. The optical properties of the antibacterial coatings were characterized by UV-VIS spectroscopy with a Jasco V-630 spectrophotometer. The samples were placed perpendicularly to the light beam during measurement, and a bare glass slide was taken as the reference for the measurements.
EDX spectra were obtained from an INCA X-ray microanalysis system from Oxford Instruments.
Bacteriologic test method
The bacteriologic tests were carried out using the standard test method  which is described in the following paragraphs. The antibacterial coatings were tested in Lactobacillus plantarum (CECT # 4005) cultures to observe their antibacterial activities. Their optimal growth conditions are 37°C, 24 h, Tryptic Soy Broth (TSB). L. plantarum stock culture was obtained from CECT (The Spanish Type Culture Collection, University of Valencia) and it was maintained by inoculating a loop onto a Tryptic Soy Agar slant and incubating at 37°C for 48 h before storing at 4-10°C.
Test samples were prepared by cutting the coated substrates into 3.5 × 3.5 cm pieces. Three separate pieces of each substrate were prepared for each bacterial strain to be evaluated. Bare glass slides were also cut and prepared following the same procedure. They were disinfected by dipping in 70% isopropyl alcohol and drying in air.
Afterwards, sterile flasks containing TSB were inoculated with the stock culture and incubated for 18 h at 37°C while shaking. From the stock culture 0.2 ml was removed and dispersed in 20 ml of sterile phosphate buffer (50 mM, pH 7.0); vortex well. Using a spectrophotometer zeroed with phosphate buffer at 600 nm, the Optical Density (OD) of the bacterial solution was read. This OD was compared with a previously developed standard curve of OD versus number of viable cells/ml to obtain the approximate number of viable cells. Then the bacterial solution was adjusted by dilution into phosphate buffer to obtain ca. 5 × 105 viable cells/ml. The obtained solution was intended to be exposed to the samples. Additionally, in order to determine the number of viable of organisms in each of the exposure solution, it was made a total of six serial 1:10 dilutions of the cell suspension (10-1, 10-2, 10-3, 10-4, 10-5, 10-6 dilution), and then it was plated 0.5 ml of the last three dilutions: 10-4, 10-5, and 10-6. They were incubated face down for 24 h at 37°C. After the incubation, it was counted the colony formation units (CFUs) and calculated the CFU/ml in all cases.
Finally, 300 μl of the adjusted bacterial suspension was applied to the plaque sample. Using sterile forceps the bacterial suspension was covered with the coated samples and the bare glass as the control sample, and carefully pressed down to ensure that the liquid spreads to all over the samples, avoiding air bubbles in theirs. Then the samples were introduced into an incubator to >90% relative humidity at 37°C for 24 h.
In order to measure the bacterial killing efficiency of the samples, the remaining bacteria were collected again using the following protocol. The samples were lifted up with forceps and TSB was repeatedly pipetted over the exposed area of the culture medium to suspend as many cells as possible. 0.5 ml of the solution was plated, and three serial 1:10 dilutions, (100, 10-1, 10-2, 10-3) onto TSA plates. Then the inoculated TSA plates were incubated for each sample, face down, at 37°C for 18 h. Finally, after the incubation, the plates was counted for the calculation of the CFU and the CFU/ml.
To measure the effect of an antimicrobial compound, the percentage of cell reduction is calculated between the control sample and the test sample:
A sample is considered biocide if the cell reduction is higher than 99% .
Results and discussion
Firstly the morphology of the thin films was studied by AFM. The resultant coating was uniform and homogeneous, showing a slightly porous surface with an average roughness of 28.3 nm (rms) (Figure 1). It has been reported in Ref.  that the basic pH of the TEOS precursor solution gives macroporous aggregates that can be assembled into a film with the dip-coating technique. This matrix shows the advantages of the inorganic materials such as mechanical strength and chemical stability, and at the same time its porosity allows the ion interchange with the external medium, a fundamental aspect when an efficient silver-based antibacterial coating is desired.
Other important aspect of the hybrid matrix is that both organic and inorganic materials should not show any phase separation, in order to get a maximum homogeneity. Other authors have reported how some polymers can interact with metal alkoxides , yielding even covalent bonding between the polymers and the inorganic material. In this work the polyelectrolyte PAA was specially selected because under certain conditions, their carboxylic groups could be eventually hydrolyzed and further covalently bonded to tetraorthosilicate particles in a sol-gel process. In a detailed AFM analysis, the phase images of the samples did not show regions with different mechanical stiffness, therefore there were not found any evidence of phase separation in the matrix.
As it has been commented in the previous section, all the coatings showed a highly transparent appearance immediately after the dip-coating fabrication step. The composition of such coatings consisted of an inorganic matrix with a small proportion of an anionic polyelectrolyte embedded within. Such polymeric chains have carboxylic functional groups that act as host sites for the silver cations during the loading immersion step by ion-interchange. Other authors have reported similar approaches to load polymeric thin films with silver ions . The visual aspect of the hybrid thin films remained unaltered after the silver loading immersion, although the silver ions were already present in the coating. However, the thin films showed a dramatic color change when they were immersed into the DMAB reducing solution. Then the samples turned almost instantaneously into a golden-yellowish color. The visual aspect of the film remained highly transparent and smooth, but with the cited color change. Such alteration of the visible absorption spectrum of the samples change is directly related with the Surface Plasmon Resonance (SPR) phenomenon [39, 40] typical of gold and silver nanoparticles. In fact, the UV-VIS absorbance spectrum confirms the existence of an absorption peak near 410 nm (Figure 2).
Such narrow absorption bands are due to the SPR phenomenon of the silver nanoparticles synthesized inside the coating. Furthermore, in order to get an additional evidence of the presence of silver within the hybrid coatings an elemental analysis was obtained using the EDX technique (Figure 3). This EDX spectrum shows a peak at 3 keV that confirms the presence of silver within the coating. The rest of the lines of the EDX spectrum correspond to other elements present in the coating (mainly Si, O, and Na) and also present in the glass slide substrate, as far as the coatings were very thin (150 nm approx.). The EDX analysis together with the SPR absorption bands of the UV-VIS spectra make possible to confirm the reduction of silver ions to elemental silver to form nanoparticles inside the organic/inorganic hybrid coating.
One of the most attractive aspects of the approach proposed in this work is that simple variations in the fabrication process can help the designer to tune the overall properties of the coating. In this work two different variations of the initial fabrication process were studied; on one hand the impact of the polyelectrolyte/TEOS ratio, and on the other hand, the number of dip/reduction cycles. The intensity of the SPR absorption band was taken as an indicator of the total amount of synthesized silver nanoparticles.
When the samples are immersed into several consecutive loading/reduction cycles the size and amount of the nanoparticles is increased . Figure 2 shows the direct relation between the number of load/reduction cycles and the increasing of the SPR absorption band around 410 nm, proportional to the amount of Ag nanoparticles trapped into the thin film. Moreover, if the concentration of the polymeric solution is varied, the silver synthesis conditions are modified. Figure 4 shows the growth of the intensity of the SPR absorption band as the number of loading/reduction cycles is increased, for two samples with different PAA molar ratio.
The results exposed in Figure 4 confirms the hypothesis that lower polyelectrolyte concentrations results in less host sites (carboxylic functional groups) for the Ag+ cations during the loading step, and after the reduction with DMAB, the amount of silver nanoparticles is significantly lower. When the same loading/reduction protocol was carried out with TEOS only coatings (without polyelectrolyte) significant absorption band was observed in the UV-VIS analysis.
Moreover, the samples were thermally treated at 450°C for 2 h to increase their mechanical stability. The resulting coatings showed a sharp improvement of the mechanical strength, and a further AFM analysis showed that there was no significant alteration in the morphology of the films. Nevertheless, the UV-VIS absorption spectra of the samples were dramatically modified. After the thermal treatment the SPR absorption peak was significantly narrowed and increased in intensity, as it is shown in Figure 5. This is consistent with the evidences found by other authors in other works .
Finally the antibacterial activities against Lactobacillus plantarum of the coatings were characterized using the method described in the "Experimental section". Figure 6 shows the results of two samples placed on agar slabs after 24 h. The first one (Figure 6a) shows a reference substrate (a bare glass slide) and it is clearly seen that a high number of Lactobacillus plantarum colonies grown up randomly throughout the whole agar slab. The second sample (Figure 6b) has a silver-loaded hybrid coated area where there is no growth of colonies. The behavior is different in the uncoated area of the substrate and in the rest of the agar slab where the growth of colonies is high as in the reference sample (Figure 6a).
All the experiments were performed in triplicate and the treated surfaces reached more than 99.9% of kill efficiency on the growth of Lactobacillus plantarum. These results confirm the high antibacterial behavior of the coatings based on silver nanoparticles polymer/sol-gel hybrid matrix.
In this work, it has been demonstrated that hybrid organic-inorganic coating matrices can be used for in situ silver nanoparticles synthesis, showing excellent antibacterial behavior against Lactobacillus plantarum. This approach is a simple and cost-effective method to get coatings with high antibacterial performance, which have most of the advantages of the inorganic coatings, like high mechanical resistance, chemical stability, etc. At the same time, the organic fraction present within the inorganic coating provides the functionality to synthesize the silver nanoparticles that gives the highly efficient antibacterial properties. This gives the ability to tune the overall properties of the film; mechanical, optical, and antibacterial.
The UV-VIS absorbance spectrum confirms the existence of silver nanoparticles inside the coating due to the presence of an absorption peak near 410 nm. Such narrow absorption bands are typical of silver nanoparticles and they are originated by the SPR phenomenon. EDX analysis also confirmed the presence of silver inside the coatings. Moreover, the impact of the organic-inorganic ratio and the number of dip-reduction cycles on the total amount of synthesized silver nanoparticles has been studied. Mechanical resistance of the coatings has been significantly improved using a thermal treatment at 450°C. This process for obtaining antibacterial surfaces can be used for different applications in a wide range of fields like in buildings, pharmaceutical tools, and other instrumental devices.
atomic force microscopy
colony formation units
energy dispersive X-ray
poly(acrylic acid sodium salt)
Surface Plasmon Resonance
Tryptic Soy Broth.
Mcdonnell G, Russell AD: Antiseptics and disinfectants: activity, action, and resistance. Clin Microbiol Rev 1999, 12: 147–179.
Russell AD: Biocide use and antibiotic resistance: the relevance of laboratory findings to clinical and environmental situations. Lancet Infect Diseases 2003, 3: 794–803. 10.1016/S1473-3099(03)00833-8
Klasen HJ: Historical review of the use of silver in the treatment of burns. I. Early uses. Burns 2000, 26: 117–130. 10.1016/S0305-4179(99)00108-4
Lansdown AB: Silver. I: Its antibacterial properties and mechanism of action. J Wound Care 2002, 11: 125–130.
Li W-R, Xie X-B, Shi Q-S, Zeng H-Y, Ou-Yang Y-S, Chen Y-B: Antibacterial activity and mechanism of silver nanoparticles on Escherichia coli . Appl Microbiol Biotechnol 2010, 85: 1115–1122. 10.1007/s00253-009-2159-5
Bragg PD, Rainnie DJ: The effect of silver ions on the respiratory chain of Escherichia coli . Can J Microbiol 1974, 20: 883–889. 10.1139/m74-135
Panáček A, Kolář M, Večeřová R: Antifungal activity of silver nanoparticles against Candida spp. Biomaterials 2009, 30: 6333–6340.
Travan A, Pelillo C, Donati I: Non-cytotoxic silver nanoparticle-polysaccharide nanocomposites with antimicrobial activity. Biomacromolecules 2009, 10: 1429–1435. 10.1021/bm900039x
Greulich C, Kittler S, Epple M, Muhr G, Köller M: Studies on the biocompatibility and the interaction of silver nanoparticles with human mesenchymal stem cells (hMSCs). Langenbeck's Arch Surg 2009, 394: 495–502.
Chen X, Schluesener HJ: Nanosilver: a nanoproduct in medical application. Toxicol Lett 2008, 176: 1–12. 10.1016/j.toxlet.2007.10.004
Yuranova T, Rincon AG, Bozzi A: Antibacterial textiles prepared by RF-plasma and vacuum-UV mediated deposition of silver. J Photochem Photobiol A 2003, 161: 27–34. 10.1016/S1010-6030(03)00204-1
Lee HY, Park HK, Lee YM, Kim K, Park SB: A practical procedure for producing silver nanocoated fabric and its antibacterial evaluation for biomedical applications. Chem Commun 2007, 2959–2961. 10.1039/b703034g
Gao Y, Cranston R: Recent advances in antimicrobial treatments of textiles. Text Res J 2008, 78: 60–72. 10.1177/0040517507082332
Blaker JJ, Nazhat SN, Boccaccini AR: Development and characterisation of silver-doped bioactive glass-coated sutures for tissue engineering and wound healing applications. Biomaterials 2004, 25: 1319–1329. 10.1016/j.biomaterials.2003.08.007
Sharma VK, Yngard RA, Lin Y: Silver nanoparticles: green synthesis and their antimicrobial activities. Adv Colloid Interface Sci 2009, 145: 83–96. 10.1016/j.cis.2008.09.002
Sharma J, Imae T: Recent advances in fabrication of anisotropic metallic nanostructures. J Nanosci Nanotechnol 2009, 9: 19–40. 10.1166/jnn.2009.J087
Wang J-X, Wen L-X, Wang Z-H, Chen J-F: Immobilization of silver on hollow silica nanospheres and nanotubes and their antibacterial effects. Mater Chem Phys 2006, 96: 90–97. 10.1016/j.matchemphys.2005.06.045
Kawashita M, Toda S, Kim H-M, Kokubo T, Masuda N: Preparation of antibacterial silver-doped silica glass microspheres. J Biomed Mater Res A 2003, 66: 266–274. 10.1002/jbm.a.10547
Rivera-Garza M, Olguín MT, García-Sosa I, Alcántara D, Rodríguez-Fuentes G: Silver supported on natural Mexican zeolite as an antibacterial material. Microporous Mesoporous Mater 2000, 39: 431–444. 10.1016/S1387-1811(00)00217-1
Park S-J, Jang Y-S: Preparation and characterization of activated carbon fibers supported with silver metal for antibacterial behavior. J Colloid Interface Sci 2003, 261: 238–243. 10.1016/S0021-9797(03)00083-3
Kawashita M, Tsuneyama S, Miyaji F, Kokubo T, Kozuka H, Yamamoto K: Antibacterial silver-containing silica glass prepared by sol-gel method. Biomaterials 2000, 21: 393–398. 10.1016/S0142-9612(99)00201-X
Jeon H-J, Yi S-C, Oh S-G: Preparation and antibacterial effects of Ag-SiO 2 thin films by sol-gel method. Biomaterials 2003, 24: 4921–4928. 10.1016/S0142-9612(03)00415-0
Bravo J, Zhai L, Wu Z, Cohen RE, Rubner MF: Transparent superhydrophobic films based on silica nanoparticles. Langmuir 2007, 23: 7293–7298. 10.1021/la070159q
Grapski JA, Cooper SL: Synthesis and characterization of non-leaching biocidal polyurethanes. Biomaterials 2001, 22: 2239–2246. 10.1016/S0142-9612(00)00412-9
Tiller JC, Lee SB, Lewis K, Klibanov AM: Polymer surfaces derivatized with poly(vinyl-N-hexylpyridinium) kill airborne and waterborne bacteria. Biotechnol Bioeng 2002, 79: 465–471. 10.1002/bit.10299
Popa A, Davidescu CM, Trif R, Ilia G, Iliescu S, Dehelean G: Study of quaternary 'onium' salts grafted on polymers: antibacterial activity of quaternary phosphonium salts grafted on 'gel-type' styrene-divinylbenzene copolymers. React Funct Polym 2003, 55: 151–158. 10.1016/S1381-5148(02)00224-9
Sunada K, Watanabe T, Hashimoto K: Studies on photokilling of bacteria on TiO 2 thin film. J Photochem Photobiol A 2003, 156: 227–233. 10.1016/S1010-6030(02)00434-3
Daniel A, Le Pen C, Archambeau C, Reniers F: Use of a PECVD-PVD process for the deposition of copper containing organosilicon thin films on steel. Appl Surf Sci 2009, 256: S82-S85. 10.1016/j.apsusc.2009.04.195
Li J, Zivanovic S, Davidson PM, Kit K: Production and characterization of thick, thin and ultra-thin chitosan/PEO films. Carbohydr Polym 2011, 83: 375–382. 10.1016/j.carbpol.2010.07.064
Yang QB, Li DM, Hong YL: Preparation and characterization of a PAN nanofibre containing Ag nanoparticles via electrospinning. Synth Met 2003, 137: 973–974. 10.1016/S0379-6779(02)00963-3
Jin W-J, Lee HK, Jeong RH, Park WH, Youk JH: Preparation of polymer nanofibers containing silver nanoparticles by using poly(N-vinylpyrrolidone). Macromol Rapid Commun 2005, 26: 1903–1907. 10.1002/marc.200500569
Marini M, De Niederhausern S, Iseppi R: Antibacterial activity of plastics coated with silver-doped organic-inorganic hybrid coatings prepared by sol-gel processes. Biomacromolecules 2007, 8: 1246–1254. 10.1021/bm060721b
Schuleit M, Luisi PL: Enzyme immobilization in silica-hardened organogels. Biotechnol Bioeng 2001, 72: 249–253. 10.1002/1097-0290(20000120)72:2<249::AID-BIT13>3.0.CO;2-B
Schultze C, Cordes A, Schmidt W, Sternberg K, Behrend D, Schmitz K-P: Hybrid polymers as implant material for medical devices. IFMBE Proc 2009, 25: 164–167. full_text
Li Z, Lee D, Sheng X, Cohen RE, Rubner MF: Two-level antibacterial coating with both release-killing and contact-killing capabilities. Langmuir 2006, 22: 9820–9823. 10.1021/la0622166
JIS Z 2801: Japanese Industrial Standard, Japanese Standard Association. 2000.
Boonamnuayvitaya V, Tayamanon C, Sae-Ung S, Tanthapanichakoon W: Synthesis and characterization of porous media produced by a sol-gel method. Chem Eng Sci 2006, 61: 1686–1691. 10.1016/j.ces.2005.10.002
Ichinose I, Kawakami T, Kunitake T: Alternate molecular layers of metal oxides and hydroxyl polymers prepared by the surface sol-gel process. Adv Mater 1998, 10: 535–539. 10.1002/(SICI)1521-4095(199805)10:7<535::AID-ADMA535>3.0.CO;2-Q
Wang TC, Cohen RE, Rubner MF: Metallodielectric photonic structures based on polyelectrolyte multilayers. Adv Mater 2002, 14: 1534–1537. 10.1002/1521-4095(20021104)14:21<1534::AID-ADMA1534>3.0.CO;2-7
Nolte AJ, Rubner MF, Cohen RE: Creating effective refractive index gradients within polyelectrolyte multilayer films: molecularly assembled rugate filters. Langmuir 2004, 20: 3304–3310. 10.1021/la0363229
Patel AC, Li S, Wang C, Zhang W, Wei Y: Electrospinning of porous silica nanofibers containing silver nanoparticles for catalytic applications. Chem Mater 2007, 19: 1231–1238. 10.1021/cm061331z
This work was supported in part by the Spanish Ministry of Education and Science CICYT-FEDER TEC 2009-09210 Research Grant. Thanks to the FIDENA foundation for the EDX measurements. Very special thanks to Paula Aldaz for her help with the bacteriologic tests.
I declare that the authors have no competing interests or other interests that might be perceived to influence the results and discussion reported in this paper.
PJR carried out the main part of the experimental work, including the fabrication of the thin films, nanoparticles synthesis, and bacteriological characterization. He participated in the design of the study and in the draft of the manuscript. AU carried the main part of the experimental work, including the fabrication of the thin films, nanoparticles synthesis, and bacteriological characterization. JG participated in the experimental work, carried out the AFM characterization of the films, and contributed with the draft of the manuscript. CRZ participated in the experimental work and carried out the EDX analysis. FJA and IRM participated in the design of the study and helped with the draft of the manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
About this article
Cite this article
Rivero, P.J., Urrutia, A., Goicoechea, J. et al. An antibacterial coating based on a polymer/sol-gel hybrid matrix loaded with silver nanoparticles. Nanoscale Res Lett 6, 305 (2011). https://doi.org/10.1186/1556-276X-6-305